Civil and Environmental Research ISSN 2224-5790 (Paper) ISSN 2225-0514 (Online) Vol.3, No.4, 2013
recycling materials as material additives. The recycling of existing asphalt pavement materials produces new pavements with considerable savings in material use, money, and energy. Aggregate and binder from old asphalt pavement retain their value even after these pavements have reached the end of their service lives (Xiao, 2009). In this study, short coconut fiber is added to asphalt heated to a certain temperature so as to avoid burning the coconut fiber. The asphalt-fiber characteristics are tested to determine such characteristics as the penetration, softening point, burning point, ductility, density, and Marshall immersion. At high temperatures, the asphalt binder tends to flow more easily due to the natural decrease in viscosity associated with higher temperatures. This condition creates a “softer” asphalt mixture, which is prone to rutting (Fontes et al, 2010). The objective of this study was to evaluate the laboratory performance of different sizes of coconut fiber present in virgin asphalt in different percentages. This goal was achieved by evaluating various engineering properties. The behavior of coconut fiber asphalt (CFA)-modified mixtures was compared to that of conventional asphalt mixtures. 2. 2.1.
Materials and methods Asphalt cement and aggregate
The aggregate used in the construction of the asphalt sample is derived from Rumpin-Bogor West Java aggregate quarry and grade 60/70 bitumen. The grading of the aggregate can be characterized as influential for the asphalt mixture deformation resistance. Poor aggregate composition refers to the use of too many fine or coarse aggregates, which fails to provide the necessary resistance to deformation. Table 1 Design aggregate gradation Sieve
In general, a higher content of fine aggregate and a perfect balance between the distribution of coarse aggregates, fine aggregate, and filler may imbue asphalt mixtures with increased resistance (Mirzahosseini et al, 2011). This study used an asphalt concrete wearing course mix (AC-WC) in which the largest aggregate size was 19 mm. The test results for the characteristics of the coarse aggregate and fine medium are displayed in Tables 1 & 2. Only one aggregate gradation shown in Figure 1 was selected for use in the study. The characteristics of asphalt must conform to the requirements specified in the Indonesian standard. Thus, tests were conducted to determine the penetration, ductility at 25 °C, loss due to heat and air, specific gravity, and softening point. The physical properties of the asphalt samples are given in Table 3.